Ab initio velocityfield curves in monoclinic β−Ga2O3 Citation ...uttamsin/JAP_2017.pdfB. Full...
Transcript of Ab initio velocityfield curves in monoclinic β−Ga2O3 Citation ...uttamsin/JAP_2017.pdfB. Full...

Ab initio velocityfield curves in monoclinic β−Ga2O3Krishnendu Ghosh and Uttam Singisetti
Citation: Journal of Applied Physics 122, 035702 (2017); doi: 10.1063/1.4986174View online: http://dx.doi.org/10.1063/1.4986174View Table of Contents: http://aip.scitation.org/toc/jap/122/3Published by the American Institute of Physics
Articles you may be interested in Highly conductive homoepitaxial Sidoped Ga2O3 films on (010) βGa2O3 by pulsed laser depositionApplied Physics Letters 111, 012103 (2017); 10.1063/1.4991363
Modulationdoped β(Al0.2Ga0.8)2O3/Ga2O3 fieldeffect transistorApplied Physics Letters 111, 023502 (2017); 10.1063/1.4993569
A correlation between the defect states and yellow luminescence in AlGaN/GaN heterostructuresJournal of Applied Physics 122, 035101 (2017); 10.1063/1.4993903
High reverse breakdown voltage Schottky rectifiers without edge termination on Ga2O3Applied Physics Letters 110, 192101 (2017); 10.1063/1.4983203
High responsivity in molecular beam epitaxy grown βGa2O3 metal semiconductor metal solar blind deepUVphotodetectorApplied Physics Letters 110, 221107 (2017); 10.1063/1.4984904
Improved performance of AlGaNbased deep ultraviolet lightemitting diodes with nanopatterned AlN/sapphiresubstratesApplied Physics Letters 110, 191103 (2017); 10.1063/1.4983283
http://oasc12039.247realmedia.com/RealMedia/ads/click_lx.ads/www.aip.org/pt/adcenter/pdfcover_test/L37/949446391/x01/AIPPT/JAP_ArticleDL_050317/PTBG_instrument_1640x440.jpg/434f71374e315a556e61414141774c75?xhttp://aip.scitation.org/author/Ghosh%2C+Krishnenduhttp://aip.scitation.org/author/Singisetti%2C+Uttam/loi/japhttp://dx.doi.org/10.1063/1.4986174http://aip.scitation.org/toc/jap/122/3http://aip.scitation.org/publisher/http://aip.scitation.org/doi/abs/10.1063/1.4991363http://aip.scitation.org/doi/abs/10.1063/1.4993569http://aip.scitation.org/doi/abs/10.1063/1.4993903http://aip.scitation.org/doi/abs/10.1063/1.4983203http://aip.scitation.org/doi/abs/10.1063/1.4984904http://aip.scitation.org/doi/abs/10.1063/1.4984904http://aip.scitation.org/doi/abs/10.1063/1.4983283http://aip.scitation.org/doi/abs/10.1063/1.4983283

Ab initio velocityfield curves in monoclinic bGa2O3Krishnendu Ghosha) and Uttam Singisettib)
Electrical Engineering Department, University at Buffalo, Buffalo, New York 14260, USA
(Received 2 June 2017; accepted 3 July 2017; published online 19 July 2017)
We investigate the highfield transport in monoclinic bGa2O3 using a combination of ab initiocalculations and full band Monte Carlo (FBMC) simulation. Scattering rate calculation and the final
state selection in the FBMC simulation use complete wavevector (both electron and phonon) and
crystal direction dependent electron phonon interaction (EPI) elements. We propose and implement
a semicoarse version of the WannierFourier interpolation method [Giustino et al., Phys. Rev. B76, 165108 (2007)] for shortrange nonpolar optical phonon (EPI) elements in order to ease thecomputational requirement in FBMC simulation. During the interpolation of the EPI, the inverse
Fourier sum over the realspace electronic grids is done on a coarse mesh while the unitary rota
tions are done on a fine mesh. This paper reports the high field transport in monoclinic bGa2O3with deep insight into the contribution of electronphonon interactions and velocityfield character
istics for electric fields ranging up to 450 kV/cm in different crystal directions. A peak velocity of
2� 107 cm/s is estimated at an electric field of 200 kV/cm. Published by AIP Publishing.[http://dx.doi.org/10.1063/1.4986174]
I. INTRODUCTION
bGa2O3 is an emerging widebandgap semiconductorwith excellent potential for power electronics applications.
Experimentally demonstrated high breakdown voltage devi
ces1–5 make it an attractive material for next generation
power electronics in addition to deep UV optoelectronic
applications.6,7 However, the low symmetry monoclinic
structure and the large primitive cell present immense chal
lenges to accurate prediction of thermal, optical, and electri
cal transport properties. There have been a number of reports
on thermal, dielectric, and optical properties of this mate
rial.8–15 Recently, we reported low field electron mobility
calculation in this material from first principles16 that fairly
agreed with experimental report.17 However, there is no
report on the high field transport properties in this material.
Highfield electron transport is important not just for elec
tronics but also for several branches of photonics. Electron
phonon interactions (EPIs) play an important role in high
field transport. It is important to have a clear quantitative
understanding of how EPIs affect highfield electron trans
port. Traditionally, they are modelled using phenomenologi
cal deformation potentials (DPs) that could explain the
experimental results. However, such an approach ignores
complex issues such as anisotropy and also requires experi
mental data to set the phenomenological constants.
Revealing the right physics of EPI is crucial to engineer the
electron and phonon dynamics. In recent years, there have
been several studies on calculating phonon scattering rates in
GaAs and Si18–22 and low field mobilites19,22 using EPI from
abinitio methods. However, including a fullband abinitiobased EPI in a Monte Carlo (MC) algorithm for high trans
port studies poses several computational challenges
especially for materials with many phonon modes. Here, we
systematically study the physics of EPI in bGa2O3 to revealhow they affect the highfield electron transport calculated
using a full band Monte Carlo (FBMC) simulation and also
address the computational challenges. Monoclinic bGa2O3has a large primitive cell with low crystal symmetry which
makes it an ideal benchmark system to study electron trans
port from first principles. The computational strategy is
discussed first followed by the results obtained for bGa2O3.
II. THEORY AND METHODS
The computation begins with the density functional the
ory (DFT) calculation on an equilibrium lattice structure
followed by the extraction of KohnSham (KS) eigen values.
Next, lattice response calculations are done based on the
density functional perturbation theory (DFPT).23 This pro
vides the dynamical phonon matrix and also the perturbation
in the selfconsistent potential for each perturbation.
Diagonalizing the dynamical phonon matrix gives the pho
non eigen values. The EPI elements are computed from
the perturbation in the selfconsistent potential.23 The EPI
elements and the phonon dynamical matrices are interpolated
using a WannierFourier interpolation scheme24 to obtain
fine sampling of the Brillouin zone. However, the longrange
polar optical phonon (POP) EPI needs a separate treatment
due to its aperiodic nature. Recent formulation25 on a long
range EPI interpolation scheme is used here.
A. Semicoarse ElectronPhonon Interaction (EPI)interpolation
The fine resolution needed on both electron (k) andphonon (q) wavevector meshes requires large memory incomputation which is exacerbated for materials with multi
ple phonon modes such as bGa2O3. Unlike scattering ratecalculations, an “on the fly” method18,26 could not be used in
the FBMC calculation since we need to store the EPI matrix
a)[email protected])[email protected]
00218979/2017/122(3)/035702/7/$30.00 Published by AIP Publishing.122, 0357021
JOURNAL OF APPLIED PHYSICS 122, 035702 (2017)
http://dx.doi.org/10.1063/1.4986174http://dx.doi.org/10.1063/1.4986174http://dx.doi.org/10.1063/1.4986174http://dx.doi.org/10.1063/1.4986174mailto:[email protected]:[email protected]://crossmark.crossref.org/dialog/?doi=10.1063/1.4986174&domain=pdf&date_stamp=20170719

elements for final state selection. An “on the fly” calculation
inside the final state selection program is inefficient since the
summation over the realspace grid has to be performed for
each electron, for each time interval, and for each scattering
process making it extremely slow. Hence, it is necessary to
store the fine grid matrix elements increasing the memory
requirement. Here, we propose a semicoarse Wannier
Fourier interpolation scheme to ease the computational
requirement of storing the finegrid matrix elements. In this
method, the unitary rotations are on a fine mesh, but the
inverse Fourier transform sum is on a coarse mesh. Storing
the finegrid electronphonon interaction (EPI) elements
requires huge runtime memory. Using the definitions of
electronic Wannier functions (WF),24 we write the short
range nonpolar EPI matrix elements on fine k and q meshesas
g�short k;qð Þ ¼1
N2eUkþq
XRe;R
0e
eik: Re�R0eð Þg�short Re �R0e;q
� �" #U†k :
(1)
Here, the unitary rotation matrices U have a dimension ofNw�Nw, where Nw is the size of the Wannier subspace.g�short k; qð Þ is the shortrange EPI on both fine meshes. Re isthe center of an unit cell in the supercell and Ne is the totalnumber of unit cells in the supercell. Eq. (1) shows the
inverse Fourier transform of the realspace (on electronic
mesh) g�short Re � R0e; q� �
to an arbitrary kpoint while theqmesh interpolated information is already present on therighthand side of the equation. The total memory require
ment to store the short range EPI on both fine meshes would
be governed by Nk x Nt x Nq x (Nw)2, which becomes largefor the required Nk and Nq where Nk, Nq, and Nt are the sizeof the fine kmesh, qmesh, and the number of phononmodes, respectively. For this work, the corresponding mem
ory requirement becomes more than 500 terabytes. Hence,
we propose a way to circumvent the problem. The primary
contribution to g�short Re � R0e; q� �
comes when the two
involved electronic WFs are on the same unit cell since the
overlap of remote WFs is low (although not negligible and
we discuss that later) in the case of maximally localized
Wannier functions (MLWFs). Under such a condition, we
can rewrite (after simple algebraic manipulation) Eq. (1) as
g�; 0short k; qð Þ ¼1
NeUkþq g
�short 0e; qð ÞU
†k
¼ UkþqU†kcþq g�;0short k ¼ kc; qð ÞUkc U
†k: (2)
Hence, the same unit cell contribution g�; 0short k; qð Þ canbe accessed just by storing g�;0short k ¼ kc; qð Þ on a coarse kmesh (kc) and the rotation matrices. This reduces thememory requirement by several orders. Next, we discuss
the contribution from remote WFs. Now, we consider Eq.
(1) with Re 6¼ R0e. Under such conditions, a reduction similar to Eq. (2) would have been perfectly possible if the
phase factor eik:ðRe�R0eÞ was absent. If the unit cells are far
enough from each other (e.g., Re � R0e >53 lattice spacing), g�short Re � R0e; q
� �becomes negligible. However, if
the unit cells are close to each other, because of the
kspace smoothness of the matrix elements in Wanniergauge, the contribution from the remote unit cells is
smaller compared to that from the same unit cell. Under
such a gaugechoice, treating the remote WF contribution
similar to Eq. (2) introduces small inaccuracy in calcula
tion but eases the computational requirement to a great
extent. So, the overall g�short k; qð Þ can be obtained fromg�short k ¼ kc; qð Þ and the rotation matrices on the fine mesh.The essential idea is to rotate the coarsemesh elements to
an optimal Blochspace that produces the maximally local
ized WF (MLWFs) and perform Fourier transform to real
space followed by inverse Fourier transform on another
coarse kmesh. The fine kmesh elements could beobtained “on the fly” just by unrotating the elements back
to the normal Blochspace using the fine kmesh rotationmatrices. This reduces the “on the fly” time consumed in
converting the elements back and forth between reciprocal
and real spaces while at the same time mitigating the huge
memory requirement for storing the elements on both fine
k and q meshes. It is important to mention here that thissacrifice of accuracy does not lead to any sacrifice of the
crystal symmetry mediated selection rules of nonpolar
scattering since that is taken care of inside short range EPI
matrix g�short Re � R0e; q� �
:
B. Full Band Monte Carlo (FBMC) simulation
Highfield transport requires Monte Carlo (MC) simula
tions. The method is widely used for velocity field curves,
and we briefly describe the method27,28,30,31 here. We solve
the Boltzmann transport equation (BTE) using the FBMC
technique starting from ab initio KS eigen values on a finereciprocal kmesh, phonon eigen values, both longrange(POP) and short range (nonpolar) EPIs, and the scattering
rates on the fine kmesh with contributions from each phonon mode treated separately. For the phonon eigen calcula
tions, we used two different types of qmeshes: one forshortrange elements that span the entire Brillouin zone
(BZ), while the other for the long range elements which exist
only in the vicinity of the zone center (ZC). Our MC scheme
is spatially homogenous, and hence, the spatial gradient term
in the BTE disappears. The ensemble of electrons is first ini
tialized in a Maxwellian thermal distribution before the elec
tric field is turned on. Electrons are allowed to drift under the
influence of the electric field and to get scattered randomly.
The free drifting of the electron changes the crystal momen
tum according to (in atomic units) _k ¼ F, where F is theapplied electric field. The free drifting time (t0) is estimated28 based on a random number r such that t0 ¼ � 1K lnr;where K is the maximum possible scattering rate from agiven band at any k point. The final state selection after ascattering mechanism is described next.
The first step of the final state selection process is to iden
tify the mechanism that caused the scattering. A “mechanism”
includes the details of phonon mode index, final electronic
band index, and the nature (polar/non polar, absorption/emis
sion) of the scattering. So, for 30 phonon modes and 2 elec
tronic bands, the allowed number of mechanisms would be
0357022 K. Ghosh and U. Singisetti J. Appl. Phys. 122, 035702 (2017)

180. It is noted that polar mechanisms do not contribute to
interband scatterings. Finding the scattering mechanism fol
lows from a normalized scattering rate (NSR) table that isformed at each k point and each band from the previouslycomputed ab initio scattering rates. The formation of the NSRtable is discussed here briefly. If Stm(k) denotes the scatteringrate of an electron at a wavevector k and an initial band mmediated by a mechanism �, the elements of the NSR table atband m and wavevector k have a form
NSR �ð Þ ¼
P�i¼1
Sim kð Þ
maxkPNmi¼1
Sim kð Þ: (3)
So, the NSR elements always lie in (0, 1) and NSR is non
decreasing with increasing �. The NSR elements are storedin a lookup table whose memory requirement scales as Nk
�Nb�Nm, where Nb is the number of bands taken in thetransport calculation and Nm is the total number of scatteringmechanisms. The large memory requirement of the NSR in a
parallel computing environment is met by storing it on
shared memory windows29 available to all processes running
under the same computing node. While selecting the mecha
nism, a random number r0 [in (0, 1)] is generated and themechanism � is selected if the relation NSR �ð Þ > r >NSR � � 1ð Þ holds true. If NSR Nmð Þ < r, the electron is“selfscattered,”27,28,30,31 which means that the state of the
electron remains unchanged.
Given an “actual” scattering event occurs, once the pho
non mode, final electronic band, and the nature of the scatter
ing are extracted from the NSR table, the next task is to findthe final electronic wavevector. We use a method tactically
similar to the one reported for covalent semiconductors29
and we treat the polar phonon mode scatterings separately.
Here, a brief detail of the algorithm is given. Let us consider
that the initial electron band index is m and wavevector iski. First, all the kpoints kj in the final band n that satisfy theenergy conservation are shortlisted. Next, a further shortlist
ing is done based on the strict energy and momentum
conservation with implementation of phonon dispersion. So
this gives a list of final kj points that satisfy both the conser
vations. Now, we exploit the fullband EPI elements and this
is where both k and q dependences of the EPI elements arerequired. Another normalized table (similar to Eq. (3)) is
formed based on the product of the local density of states
(LDOS) at the potential kjs and EPI strength at the corre
sponding momentum conserving phonon wavevector, qj.
This is where the polar scattering needs to be taken care of
separately. The smallangle preference of the polar mecha
nisms needs to be properly captured in order to reflect the
lower momentum relaxation time compared to corresponding
energy relaxation time. This is done with the aid of a sepa
rate fine qmesh that exists only near the zone center. Usinga random number, the normalized table is scanned through
like it was done for NSR and a final kj is selected. However,
this only gives the grid point in the reciprocal space. The
final electron wavevector could belong to anywhere within
the small cube that is represented by this grid point. The
scheme to select the final wavevector within the small cube
is exactly the same as the one described in steps (e)–(g) of
Fig. 7 in Ref. 29. Next, we discuss the calculation and results
for bGa2O3.
III. RESULTS AND DISCUSSION
We carry out DFT calculations on bGa2O3 as describedin our previous work16 with similar pseudopotentials35 and
zone sampling36 using Quantum ESPRESSO.37 Figure 1(a)
shows the crystal structure of bGa2O3 along with theCartesian direction convention that is followed throughout
this work. In Fig. 1(b), we show the resulting KS eigen val
ues along two reciprocal vectors. Four conduction bands are
shown out of which the first two are used in subsequent
transport calculations. Figure 1(c) shows the equienergy
surfaces for two different energies. It can be seen that at a
lower energy the surface is spherically symmetric, while at
higher energies the surface becomes anisotropic with contri
butions from higher energy bands. We interpolated the KS
Hamiltonian through MLWFs by using the wannier90
FIG. 1. (a) Crystal structure of bGa2O3. a, b, and c represent the conventional lattice directions for monoclinic
crystals. The Cartesian x, y, and z directions used for the calculations are also
shown. (b) The DFT calculated conduc
tion band energies are shown for bGa2O3. The first two bands (shown in
red and blue) are used in the transport
calculation. (c) The equienergy surfa
ces are shown for two different energies.
It is evident that at lower energy the sur
face is spherically symmetric while
higher energy introduces band anisot
ropy and also multiple bands. (a) is visu
alized by Vesta32,33 and (c) is visualized
by XcrySDen.34
0357023 K. Ghosh and U. Singisetti J. Appl. Phys. 122, 035702 (2017)

code.38 Our optimal Wannier subspace (S) consists of two
low lying conduction bands within a frozen energy window.
The phonon calculation is done under DFPT using QE. The
phonon eigen values and the shortrange (nonpolar) EPI
matrix elements are interpolated on a fine qmesh using amodified version of the EPW code.26
A. EPI in bGa2O3
The shortrange nonpolar EPI elements are primarily
responsible for higher momentum and energy relaxation
rates at highfields that lead to saturation in velocity. The
WannierFourier interpolated shortrange matrix elements
are shown in Fig. 2(a) with respect to q. We show the sum ofthe squared magnitude of the coupling over all the vibra
tional modes. The longrange POP coupling is also shown on
the same plot for comparison. The q dependence of EPImatrix elements ð
Pt jgtshortj
2Þ is to be noted along with itscrystal direction dependence (CZ and CN), and the strengthis minimized at the C point. The inset shows a contour ploton the 2D plane formed by the same two directions. The
symmetry of the shortrange element observed on the con
tour plot is a signature of the inversion symmetry associated
with the C2m space group.39 The small discontinuity on the
shortrange EPI marked by the arrow is a result of the gauge
ambiguity arising from degenerate final electronic states [see
Fig. 1(b)]. Such discontinuity does not affect the total scat
tering rate since the latter is gaugeinvariant. Figure 2(b)
shows the shortrange EPI for each phonon mode for two dif
ferent q vectors. The red bars show jgtshortj2
for initial elec
tron wavevector k at 0.25�CZ away from C while thephonon wavevector (q) is 0.5�CZ away from C. The corresponding two points from the green bars are 0.125�CN (k)away from C and 0.25�CN (q) away from C. The inset ofFig. 2(b) shows the scattering schematic for high energy
electrons. The long arrows correspond to a direction reversal
of an electron which provides a high momentum relaxation.
For highfield transport, the available phase space allows
phonon wavevectors from all directions. But the higher
momentum relaxing phonon wavevectors need to be
inclined as much opposite as possible to the propagating
electron wavevector. This explains the choice of electron
and phonon wavevectors to show the individual mode con
tributions in Fig. 2(b). It could be seen that for an electron
with initial wavevector at the C point, the dominating nonpolar phonon modes are at 83 and 96 meV along CZ, whilealong CN, they are 22 and 90 meV. Figure 2(c) shows theshort range EPI element (g�short kð Þ) along the CZC directioncalculated using the coarse mesh, fine mesh, and semicoarse
sampling proposed in this work. The q vector for these calculations is kept fixed at halfway along the CZ. The DFPTcalculated coarsemesh element is shown with red dots,
while a regular fine mesh interpolated result is shown with a
red solid curve. The kinks on the semicoarse curves occur
when the representative coarse kmesh point correspondingto a finek mesh point changes. The small errors incurreddue to this strategy are acceptable given the resulting ease in
computational memory requirement. The key aspect is that
the coarse mesh used in the Fourier transform does not have
to be as coarse as the original DFT mesh. It should be made
as fine as possible within the available computational resour
ces. The maximum observed deviation between the 8� 8� 4semicoarse mesh and the fine mesh elements is �12% alongthe CZC direction for this given q vector.
B. Scattering rates and highfield transport
Next, we discuss the FermiGolden rule computed non
polar phonon scattering rates. The energy conserving delta
function is implemented using a Lorentzian smearing. We
carried out an analytical fitting of the computed scattering
rates using a deformation potential (DP) approximation31 to
guide future analytical transport calculations. However, it is
important to note that resulting fitting parameters do not
provide any actual physical picture of EPI or existence of
phonon modes. The density of states used in the scattering
rate fitting procedure is computed from the ab initio bandstructure. For nonpolar optical phonon scattering [Fig. 3(a)],
we fitted the computed scattering rates with D02/x0¼ 7.2
� 1018 eV/cm2, where D0 is the optical deformation potentialand x0 is the optical phonon energy. For a suitable fitting,these two parameters are interadjustable and hence are not
FIG. 2. (a) The dependence of the EPI elements with the phonon wavevector (q). The inset shows a contour plot of the shortrange EPI on the CZCN plane.The initial electronic state is taken at the C, and hence, the inversion symmetry of the crystal is reflected in the contour plot. (b) The modewise splitting of theshortrange EPI for two q points along two different directions. The phonon energies (meV) for the dominating modes are shown with corresponding colors.(Inset) At higher electron energies, a high momentum relaxation requires phonon wavevectors that are inclined towards the opposite direction of the electronic
wavevector. (c) The interpolated elements in kspace using the semicoarse kmesh strategy. The q point is kept fixed at a point halfway along CZ. A purefinemesh interpolation is also shown for comparison. In (a)–(c), the initial and final electronic band indices are taken to be the first band.
0357024 K. Ghosh and U. Singisetti J. Appl. Phys. 122, 035702 (2017)

unique. Figure 3(a) shows the fitted curves with dashed
curves. Figure 3(b) shows the calculated acoustic phonon
scattering rate with energy. For acoustic phonons, the fitting
procedure is twofold as seen in Fig. 3(b). Scattering due to
the zonecenter (ZC) phonons is fitted with DA2/vs
2
¼ 5� 10�11 eV2 s2/cm2, where DA is the acoustic deformation potential and vs is the velocity of sound. On the other
hand, the zoneedge (ZE) acoustic phonons have a dispersion
similar to optical phonons; hence, we use an optical phonon
like fitting with DAZE¼ 5� 107 eV/cm and xAZE¼ 0.01 eV
[dashed green lines in Fig. 3(b)]. A single fitting of the
acoustic scattering rate is not possible because of the approx
imations31 used to derive the analytical form of the scattering
rate, namely, the negligible phonon energy and the linear
dependence of the coupling with phonon wavevector.
Now, we discuss the results of the Monte Carlo simula
tion. Figure 4(a) shows the initialized Maxwell electron dis
tribution in energy space at room temperature at the start of
the FMBC simulation, while Fig. 4(b) shows the initial elec
tron distribution along kz in the direction (zdirection) of theapplied electric field. The respective bottom panels [Figs.
4(c) and 4(d)] show similar plots for an applied electric field
of 300 kV/cm along the z direction. It is noted that the nonequilibrium distribution in energy space dies off well beyond
2 eV of energy. The first satellite valley occurs at �2.5 eV;hence, very few electrons are transferred to satellite valleys
at the field strength. This is further supported by the electron
distribution as a function of kz seen in Fig. 4(d), which showsvery low population near the zone edge where the valley
occurs. Next, we discuss the transient response of the drift
velocity as shown in Fig. 5. At low electric fields, the trans
port is dominated by POP scattering and the momentum
relaxation rate is not increasing with electron energy imply
ing that the drift velocity monotonically arrives to a steady
state. However, beyond 150 kV/cm velocity, overshoot starts
to appear. This is attributed to the fact that with increasing
electron energy, the intraband nonpolar scattering becomes
significantly high allowing shortrange transitions that boost
up momentum relaxation drastically while the energy relaxa
tion is still limited by the energy of the phonon modes. The
imbalance of the two rates results31 in a slow rise of the elec
tron energy than the same in the drift velocity. However, the
momentum relaxation rate is also dependent on the electron
energy and hence it gets adjusted in a larger timescale than
that of the drift velocity and hence we see the overshoot.
Figure 6 shows the velocityfield curves in three differ
ent Cartesian directions calculated from FBMC using the
FIG. 3. (a) Comparison of computed nonpolar optical phonon (NOP) scat
tering rate and fitted NOP scattering rate. (b) Comparison of computed
acoustic phonon scattering rate with the corresponding fittings. The fitting
splits the contribution from zonecenter and zone edge acoustic modes. See
text for fitting parameters.
FIG. 4. Electron population in energy
space and kz space. (a) and (b) showthe histogram plots for initial condi
tions used in the FBMC simulation and
(c) and (d) show the corresponding
plots for the steady state under an
external electric field of 300 kV/cm
applied along the z direction.
0357025 K. Ghosh and U. Singisetti J. Appl. Phys. 122, 035702 (2017)

scattering strengths discussed in Secs. II and III A. We see
that the velocity increases in all three directions up to
200 kV/cm followed by a negative differential conductivity
(NDC). The calculated NDC is less than that observed in
GaAs since the satellite valleys occur at a much higher
energy (the lowest one being at�2.4 eV) as compared toGaAs (�0.3 eV). Unlike GaAs and GaN where the NDCresults from intervalley scattering, the NDC and velocity
saturation in bGa2O3 result from intravalley shortrangescattering. In bGa2O3, the nonparabolic nature of the C valley at higher electronic energies reduces the average elec
tronic group velocities resulting in the NDC and the short
range intravalley EPI results in the saturation of velocity.
For the range of electric fields considered here, electrons
barely reach the satellite valleys [see Fig. 4(c)]. So, the fact
that the velocity starts rolling off from its peak value beyond
200 kV/cm is to be attributed to the nonparabolicity of the
conduction band rather than intervalley scatterings. The
average peak velocity at an electric field of 200 kV/cm
is�2� 107 cm/s which is slightly lower than that of wurtziteGaN.40 Next, we discuss the observed anisotropy in the
velocityfield curves. Prior to the peak velocity point, around
100 kV/cm, the z direction velocity is lower than that in xand y directions. This is attributed to the large polar opticalphonon scattering by the Bu
1 mode which is polarized in the
z direction as was observed in our previous work.16 Moredetails on this anisotropy could be found in a future work.41
However, beyond the peak velocity, the drift velocity is rela
tively higher in the y direction. We attribute this to the fact
that the slope of the energy band drops at a higher k in the ydirection compared to that in the other two directions.
Hence, the ensemble average of the drift velocity is higher in
the y direction. The velocityfield curves were fitted using
the Barnes model42 that formulates NDC with, ln Fð Þ
¼ l0þvsat
FF
Fcð Þc
1þ FFcð Þc , where l0 is the lowfield mobility and vsat, Fc,
and c are the adjustable fitting parameters. This model isused in commercial device simulators43 to simulate device
operation. The fitting parameters in three different directions
are given in Table I. It is noted that, these parameters are
good only up to an electric field of about 500 kV/cm.
Beyond that, other physical phenomena such as interband
transitions and impact ionization are likely to kick in which
will modify the velocityfield curves.
IV. SUMMARY
In summary, we have highlighted the role of fullband
EPI in controlling the electron transport in bGa2O3. A semicoarse kmesh version of the WannierFourier interpolation24 strategy is proposed for the shortrange EPI in order to
make it computationally tractable in a Monte Carlo algo
rithm. The applicability of this strategy is valid within the
current scope of this work; however, for validating this
method for arbitrary material systems, further study is
required which itself could be a topic for future work. The
calculated EPIs are used in an FBMC algorithm to analyze
highfield transport. Scattering rate fitting parameters are cal
culated to guide analytical calculations. Monoclinic bGa2O3is studied under this theoretical manifold followed by the
prediction of the velocityfield characteristics. The velocity
field curves are fitted in different directions using compact
NDC models to guide device design.
ACKNOWLEDGMENTS
The authors acknowledge the support from the National
Science Foundation (NSF) Grant (No. ECCS 1607833). The
authors also acknowledge the excellent high performance
computing cluster provided by the Center for Computational
Research (CCR) at the University at Buffalo.
1M. Higashiwaki, K. Sasaki, T. Kamimura, M. Hoi Wong, D.
Krishnamurthy, A. Kuramata, T. Masui, and S. Yamakoshi, “Depletion
mode Ga2O3 metaloxidesemiconductor fieldeffect transistors on bGa2O3 (010) substrates and temperature dependence of their device char
acteristics,” Appl. Phys. Lett. 103(12), 123511 (2013).2M. Higashiwaki, K. Sasaki, A. Kuramata, T. Masui, and S. Yamakoshi,
“Gallium oxide (Ga2O3) metalsemiconductor fieldeffect transistors on
singlecrystal bGa2O3 (010) substrates,” Appl. Phys. Lett. 100(1), 013504(2012).
FIG. 5. Transient response of drift velocity for different electric fields.
FIG. 6. Velocityfield characteristic of bGa2O3 at room temperature in threedifferent directions.
TABLE I. Analytical fitting parameters for the computed velocityfield
curves.
x y z
l0 (cm2/V s) 140 140 112
vsat (cm/s) 107 1.5 � 107 107
Fc (V/cm) 2.25 � 105 1.54 � 105 2.63 � 105
c 2.84 2.47 3.35
0357026 K. Ghosh and U. Singisetti J. Appl. Phys. 122, 035702 (2017)
http://dx.doi.org/10.1063/1.4821858http://dx.doi.org/10.1063/1.3674287

3T. Oishi, Y. Koga, K. Harada, and M. Kasu, “Highmobility bGa2O3 201single crystals grown by edgedefined filmfed growth method and their
Schottky barrier diodes with Ni contact,” Appl. Phys. Express 8(3),031101 (2015).
4K. Sasaki, M. Higashiwaki, A. Kuramata, T. Masui, and S. Yamakoshi,
“Schottky barrier diodes fabricated by using singlecrystal bGa2O3 (010)substrates,” IEEE Electron Device Lett. 34(4), 493–495 (2013).
5K. Zeng, K. Sasaki, A. Kuramata, T. Masui, and U. Singisetti, “Depletion
and enhancement mode bGa2O3 MOSFETs with ALD SiO2 gate and near400 V breakdown voltage,” in 74th Annual Device Research Conference(DRC) (IEEE, 2016), pp. 1–2.
6S. Nakagomi, T. Momo, S. Takahashi, and Y. Kokubun, “Deep ultraviolet
photodiodes based on bGa2O3/SiC heterojunction,” Appl. Phys. Lett.103(7), 072105 (2013).
7T. Oshima, T. Okuno, N. Arai, N. Suzuki, S. Ohira, and S. Fujita,
“Vertical solarblind deepultraviolet Schottky photodetectors based on
bGa2O3 substrates,” Appl. Phys. Express 1(1), 011202 (2008).8B. Liu, M. Gu, and X. Liu, “Lattice dynamical, dielectric, and thermody
namic properties of bGa2O3 from first principles,” Appl. Phys. Lett.91(17), 172102 (2007).
9Z. Guo, A. Verma, X. Wu, F. Sun, A. Hickman, T. Masui, A. Kuramata,
M. Higashiwaki, D. Jena, and T. Luo, “Anisotropic thermal conductivity in
single crystal bgallium oxide,” Appl. Phys. Lett. 106(11), 111909 (2015).10M. Schubert, R. Korlacki, S. Knight, T. Hofmann, S. Sch€oche, V.
Darakchieva, E. Janz_en, B. Monemar, D. Gogova, Q. T. Thieu, R. Togashi,
H. Murakami, Y. Kumagai, K. Goto, A. Kuramata, S. Yamakoshi, and M.
Higashiwaki, “Anisotropy, phonon modes, and free charge carrier parameters
in monoclinic bgallium oxide single crystals,” Phys. Rev. B 93(12), 125209(2016).
11Y. Zhang, J. Yan, G. Zhao, and W. Xie, “Firstprinciples study on elec
tronic structure and optical properties of Sndoped bGa2O3,” Phys. B:Condens. Matter 405(18), 3899–3903 (2010).
12S. Badescu, D. Thomson, J. Mann, and G. Jessen, “Atomistic modelling
for predicting bGa2O3 properties,” paper presented at the 1st InternationalWorkshop on Gallium Oxide and Related Materials, Kyoto University,
Kyoto, Japan (2015).13M. Schubert, “Coordinateinvariant LyddaneSachsTeller relationship for
polar vibrations in materials with monoclinic and triclinic crystal sys
tems,” Phys. Rev. Lett. 117(21), 215502 (2016).14F. Ricci, F. Boschi, A. Baraldi, A. Filippetti, M. Higashiwaki, A.
Kuramata, V. Fiorentini, and R. Fornari, “Theoretical and experimental
investigation of optical absorption anisotropy in bGa2O3,” J. Phys.:Condens. Matter 28(22), 224005 (2016).
15K. A. Mengle, G. Shi, D. Bayerl, and E. Kioupakis, “Firstprinciples calcu
lations of the nearedge optical properties of bGa2O3,” Appl. Phys. Lett.109(21), 212104 (2016).
16K. Ghosh and U. Singisetti, “Ab initio calculation of electronphonon couplingin monoclinic bGa2O3 crystal,” Appl. Phys. Lett. 109(7), 072102 (2016).
17A. Parisini and R. Fornari, “Analysis of the scattering mechanisms control
ling electron mobility in bGa2O3 crystals,” Semicond. Sci. Technol.31(3), 035023 (2016).
18M. Bernardi, D. VigilFowler, C. S. Ong, J. B. Neaton, and S. G. Louie,
“Ab initio study of hot electrons in GaAs,” Proc. Natl. Acad. Sci. U. S. A.112(17), 5291–5296 (2015).
19J.J. Zhou and M. Bernardi, “Ab initio electron mobility and polar phononscattering in GaAs,” Phys. Rev. B 94(20), 201201 (2016).
20M. Bernardi, D. VigilFowler, J. Lischner, J. B. Neaton, and S. G. Louie,
“Ab initio study of hot carriers in the first picosecond after sunlight absorption in silicon,” Phys. Rev. Lett. 112(25), 257402 (2014).
21J. Zhou, B. Liao, and G. Chen, “Firstprinciples calculations of thermal,
electrical, and thermoelectric transport properties of semiconductors,”
Semicond. Sci. Technol. 31(4), 043001 (2016).22J. Sjakste, N. Vast, M. Calandra, and F. Mauri, “Wannier interpolation of
the electron phonon matrix elements in polar semiconductors: Polar
optical coupling in GaAs,” Phys. Rev. B 92, 054307 (2015).
23A. D. C. S. Baroni and S. De. Gironcoli, “Phonons and related crystal
properties from densityfunctional perturbation theory,” Rev. Mod. Phys.
73, 515–562 (2001).24F. Giustino, M. L. Cohen, and S. G. Louie, “Electronphonon interaction
using Wannier functions,” Phys. Rev. B 76(16), 165108 (2007).25C. Verdi and F. Giustino, “Frohlich electronphonon vertex from first
principles,” Phys. Rev. Lett. 115(17), 176401 (2015).26J. Noffsinger, F. Giustino, B. D. Malone, C.H. Park, S. G. Louie, and M.
L. Cohen, “EPW: A program for calculating the electronphonon coupling
using maximally localized Wannier functions,” Comput. Phys. Commun.
181(12), 2140–2148 (2010).27D.Vasileska and S. M. Goodnick, see https://nanohub.org/resources/9109
for Bulk Monte Carlo: Implementation details and source codes download,
2010.28C. Jacoboni and L. Reggiani, “The Monte Carlo method for the solution of
charge transport in semiconductors with applications to covalent materi
als,” Rev. Mod. Phys. 55(3), 645 (1983).29MPI: A messagepassing interface standard version 3.0, 2012.30T. Kunikiyo, M. Takenaka, Y. Kamakura, M. Yamaji, H. Mizuno, M.
Morifuji, K. Taniguchi, and C. Hamaguchi, “A Monte Carlo simulation
of anisotropic electron transport in silicon including full band structure
and anisotropic impactionization model,” J. Appl. Phys. 75(1), 297(1994).
31M. Lundstrom, Fundamentals of Carrier Transport (CambridgeUniversity Press, 2009).
32K. Momma and F. Izumi, “VESTA: A threedimensional visualization
system for electronic and structural analysis,” J. Appl. Crystallogr. 41(3),653–658 (2008).
33See http://www.misasa.okayamau.ac.jp/�masami/vesta/Ga2O3beta.vesta for the cif file for bGa2O3.
34A. Kokalj, “Computer graphics and graphical user interfaces as tools in
simulations of matter at the atomic scale,” Comput. Mater. Sci. 28(2),155–168 (2003).
35J. P. Perdew and Y. Wang, “Accurate and simple analytic representation
of the electron gas correlation energy,” Phys. Rev. B 45(23), 13244–13249(1992).
36H. J. Monkhorst and J. D. Pack, “Special points for Brillouinzone integra
tions,” Phys. Rev. B 13(12), 5188–5192 (1976).37P. Giannozzi, S. Baroni, N. Bonini, M. Calandra, R. Car, C. Cavazzoni, D.
Ceresoli, G. L. Chiarotti, M. Cococcioni, I. Dabo, A. Dal Corso, S. de
Gironcoli, S. Fabris, G. Fratesi, R. Gebauer, U. Gerstmann, C.
Gougoussis, A. Kokalj, M. Lazzeri, L. MartinSamos, N. Marzari, F.
Mauri, R. Mazzarello, S. Paolini, A. Pasquarello, L. Paulatto, C. Sbraccia,
S. Scandolo, G. Sclauzero, A. P. Seitsonen, A. Smogunov, P. Umari, and
R. M. Wentzcovitch, “Quantum espresso: A modular and opensource
software project for quantum simulations of materials,” J. Phys. Condens.
Matter 21(39), 395502 (2009).38A. A. Mosto_, J. R. Yates, Y.S. Lee, I. Souza, D. Vanderbilt, and N.
Marzari, “Wannier90: A tool for obtaining maximally localised Wannier
functions,” Comput. Phys. Commun. 178(9), 685–699 (2008).39See http://homepage.univie.ac.at/nikos.pinotsis/spacegroup.html#12 for
the 4 symmetry operations are identity, inversion, 2fold rotation around
the unique axis, and a mirror symmetry across the plane perpendicular to
the unique axis.40J. Kolnik, I. H. O. Guzman, K. F. Brennan, R. Wang, P. P. Ruden, and Y.
Wang, “Electronic transport studies of bulk zincblende and wurtzite
phases of GaN based on an ensemble Monte Carlo calculation including a
full zone band structure,” J. Appl. Phys. 78(2), 1033–1038 (1995).41K. Ghosh and U. Singisetti, “Anisotropy of electron transport in mono
clinic bGa2O3 crystal” (unpublished).42J. J. Barnes, R. J. Lomax, and G. I. Haddad, “Finiteelement simulation of
GaAs MESFET’s with lateral doping profiles and submicron gates,” IEEE
Trans. Electron Devices 23(9), 1042–1048 (1976).43Atlas, Device Simulator. “Atlas user’s manual.” Silvaco International
Software, Santa Clara, CA, USA (2016).
0357027 K. Ghosh and U. Singisetti J. Appl. Phys. 122, 035702 (2017)
http://dx.doi.org/10.7567/APEX.8.031101http://dx.doi.org/10.1109/LED.2013.2244057http://dx.doi.org/10.1063/1.4818620http://dx.doi.org/10.1143/APEX.1.011202http://dx.doi.org/10.1063/1.2800792http://dx.doi.org/10.1063/1.4916078http://dx.doi.org/10.1103/physrevb.93.125209http://dx.doi.org/10.1016/j.physb.2010.06.024http://dx.doi.org/10.1016/j.physb.2010.06.024http://dx.doi.org/10.1103/PhysRevLett.117.215502http://dx.doi.org/10.1088/09538984/28/22/224005http://dx.doi.org/10.1088/09538984/28/22/224005http://dx.doi.org/10.1063/1.4968822http://dx.doi.org/10.1063/1.4961308http://dx.doi.org/10.1088/02681242/31/3/035023http://dx.doi.org/10.1073/pnas.1419446112http://dx.doi.org/10.1103/PhysRevB.94.201201http://dx.doi.org/10.1103/PhysRevLett.112.257402http://dx.doi.org/10.1088/02681242/31/4/043001http://dx.doi.org/10.1103/PhysRevB.92.054307http://dx.doi.org/10.1103/RevModPhys.73.515http://dx.doi.org/10.1103/PhysRevB.76.165108http://dx.doi.org/10.1103/PhysRevLett.115.176401http://dx.doi.org/10.1016/j.cpc.2010.08.027https://nanohub.org/resources/9109http://dx.doi.org/10.1103/RevModPhys.55.645http://dx.doi.org/10.1063/1.355849http://dx.doi.org/10.1107/S0021889808012016http://www.misasa.okayamau.ac.jp/~masami/vesta/Ga2O3beta.vestahttp://www.misasa.okayamau.ac.jp/~masami/vesta/Ga2O3beta.vestahttp://www.misasa.okayamau.ac.jp/~masami/vesta/Ga2O3beta.vestahttp://dx.doi.org/10.1016/S09270256(03)001046http://dx.doi.org/10.1103/PhysRevB.45.13244http://dx.doi.org/10.1103/PhysRevB.13.5188http://dx.doi.org/10.1088/09538984/21/39/395502http://dx.doi.org/10.1088/09538984/21/39/395502http://dx.doi.org/10.1016/j.cpc.2007.11.016http://homepage.univie.ac.at/nikos.pinotsis/spacegroup.html#12http://dx.doi.org/10.1063/1.360405http://dx.doi.org/10.1109/TED.1976.18533http://dx.doi.org/10.1109/TED.1976.18533
s1s2s2Aln1n2d1d2s2Bd3s3f1s3As3Bf2f3f4s4c1c2f5f6t1c3c4c5c6c7c8c9c10c11c12c13c14c15c16c17c18c19c20c21c22c23c24c25c26c27c28c29c30c31c32c33c34c35c36c37c38c39c40c41c42c43